Lanthanum sulfide/graphene oxide composite thin films and their supercapacitor application
- 169 Downloads
In this study, graphene oxide, lanthanum sulfide and their composite thin films are prepared using simple and inexpensive chemical methods and their supercapacitive performance is evaluated. The X-ray diffraction study shows the formation of mixed-phase lanthanum sulfide with monoclinic α-LaS2 and tetragonal La5S7. Field emission scanning electron microscopy images show porous surface morphology of lanthanum sulfide and composite thin films. The supercapacitive performance of composite film tested in 1 M Na2SO4 electrolyte shows highest specific capacitance of 312 F g−1 at a 5 mV s−1 scan rate.
KeywordsGraphene oxide Lanthanum sulfide Successive ionic layer adsorption reaction Supercapacitor Thin films
Electrochemical energy storage is a high requirement for intermittent renewable energy sources. The energy storage devices mainly include lithium-ion batteries and supercapacitors [1, 2]. The energy storage in the supercapacitor is established by two mechanisms. One is the electrical double-layer capacitive (EDLC) and another one is the pseudocapacitive. Electrical double-layer capacitors (EDLC) based on quick ion adsorption/desorption and pseudocapacitors originated from fast faradaic charge transfer reactions occurred at electrode surface [3, 4]. Earlier used pseudocapacitive materials were transition metal oxides and conducting polymers having both the improved energy and power densities [5, 6].
Lanthanum sulfide is one of the promising rare earth materials used recently as supercapacitor electrode. The films of lanthanum sulfide with phase of α-La2S3 are prepared using successive ionic layer adsorption and reaction (SILAR) method by Patil et al.  who showed maximum capacitance of 256 F g−1. Patil et al.  studied the effect of aqueous electrolyte on the performance of La2S3 films. Also, Ghogare et al.  prepared β-LaS2 film by hydrothermal method and reported a specific capacitance of 121.42 F g−1. Lanthanum sulfide electrode showed good energy storage capacity in both aqueous and non-aqueous electrolytes .
Graphene oxide (GO) is more motivating because of its monolayer arrangement of carbon atoms in a honeycomb network with SP2 bonding configuration . The GO-based materials provide high surface area backbone metal oxides/sulfides that increase capacitance of GO-based composite electrode through faradaic reactions . The GO is one of the most important derivatives of graphene, which is characterized by a layered structure with oxygen functional group attached on the basal planes and edges because of which GO has the hydrophilic nature, so that water dispersion of GO provides an easy path for preparing its composite with metal sulfides [13, 14].
This article reports for the first time the preparation of lanthanum sulfide/GO composite thin films prepared by successive ionic layer adsorption and reaction method on a stainless steel substrate. The GO is deposited using layer-by-layer (LBL) deposition method. For a preparation of composite film, lanthanum sulfide electrode is deposited onto GO. The structural and morphological analyses of these films are carried out using XRD and FE-SEM techniques. Further, the electrodes are studied for supercapacitive application in 1 M Na2SO4 electrolyte.
2.1 Synthesis of GO thin films
The GO was synthesized from graphite flakes by a modified Hummers method [15, 16]. Typically, graphite (5 g) and NaNO3 (2.5 g) were mixed with 120 ml of H2SO4 (95%) in a 500-ml flask. The mixture was stirred for 30 min in an ice-water bath. While maintaining vigorous stirring, potassium permanganate (15 g) was added to the suspension slowly to keep the reaction temperature below 20 °C. Upon completion of potassium permanganate addition, the ice-water bath was removed, and the mixture was kept stirring at room temperature for overnight. As the reaction proceeded, the mixture gradually became pasty, and the color turned into light brownish. After overnight stirring, 150 ml double-distilled water (DDW) was slowly added to the paste with vigorous agitation while the paste color changed to yellow. The diluted suspension was stirred for another 15 min, and 50 ml 30% H2O2 was added to the mixture. For purification, the mixture was washed with DDW for several times until pH 7 is achieved. After filtration, brownish-colored GO was obtained.
For the preparation of GO thin films, layer-by-layer (LBL) method was used. The prepared GO of 1 mg ml−1 was exfoliated in 120 ml DDW using ultrasonic treatment for 1 h. This process provided a well-dispersed brown-colored solution of GO sheets. A 40-ml GO from this solution was taken and the cleaned glass and stainless steel substrate were immersed and kept for 40 s, then withdrawn gradually and dried with air drier for 20 s, to improve the adherence of GO sheets to the substrate. Such 100 cycles were repeated to achieve the optimum thickness of GO films.
2.2 Synthesis of lanthanum sulfide thin film
The deposition of lanthanum sulfide thin film by SILAR method comprises the successive immersion of the substrate in cationic precursor and anionic precursor solutions at room temperature. An aqueous 0.1 M LaCl3·7H2O solution is used as the cationic precursor, and 0.05 M Na2S solution was utilized as the anionic precursor. The cleaned stainless steel substrate is immersed in the cationic precursor for 20 s, and La+3 ions are adsorbed on the substrate, followed by 10-s rinsing in DDW to remove the loosely bound species of La+3. Successively, the substrate is dipped into the anionic precursor solution for 20 s to build a layer of lanthanum sulfide. Again, the substrate is rinsed for 10 s in DDW to take out the overloaded or unreacted species. In this way, one SILAR cycle of lanthanum sulfide deposition is completed and 100 such deposition cycles are reiterated to get the terminal thickness of the film.
2.3 Synthesis of composite thin film
For the fabrication of composite thin films, the prepared GO solution is used as the source of GO sheets; cationic precursor solution is 0.1 M LaCl3·7H2O, and 0.05 M Na2S is an anionic precursor solution. The single layer of composite film through LBL and SILAR methods is deposited using the procedure as follows. The well-cleaned stainless steel substrate is immersed in a solution of GO for 40 s and then air-dried for 20 s for GO sheets deposition on the substrate. Then, the substrate is dipped in the cationic precursor solution for 20 s for the adsorption of lanthanum species on the GO sheets. Then, the substrate is rinsed in DDW for 10 s to remove loosely bound species of La+3 species. After, the substrate is immersed in the anionic precursor solution (S−2) for 20 s to form a layer of lanthanum sulfide material on GO sheets. Again, the substrate is rinsed in DDW for 10 s to separate out the overload or unreacted species. Thus, one cycle of the composite deposition is completed and 100 such deposition cycles are repeated to achieve an optimum thickness of the film. The loading GO on stainless steel is 0.069 gm cm−2 and loading of lanthanum sulfide is 0.083 gm cm−2 in composite film.
2.4 Materials characterization
The crystal structure of GO, lanthanum sulfide and composite thin film was examined using a Bruker AXS D8 advance model X-ray diffractometer with primary monochromatic radiation from Cu Kα line (λ = 1.54 Å) in the 2θ range of 10–80°. The surface morphology of thin films was observed using field emission scanning electron microscope (FE-SEM, JEOL-6360, Japan). The wettability test was conducted by contact angle measurement (water as a solvent) using Rame-Hart NRL CA Goniometer. Electrochemical measurements of GO, lanthanum sulfide and composite thin films were taken using Zive MP1 model of Wonatech company using three-electrode cell, consisting of thin films as the working electrode, platinum as a counter electrode and the saturated calomel electrode (SCE) as a reference electrode.
3 Results and discussion
Electrochemical impedance spectroscopy (EIS) technique is used for GO, lanthanum sulfide and composite electrodes studies in 1 M Na2SO4 electrolyte. The power output capability of supercapacitors strongly depends on the impedance of the electrode. The total impedance of the supercapacitor consists of electronic and ionic contributions. The previous is related to the intrinsic electronic resistance of the electrode particles and the interfacial resistances of particles-to-particles and particles-to-current collector. The second one is associated with the electrolyte resistance in the pores and the ionic (diffusion) resistance of ions moving in the small pores. The porosity of electrode results in the distorted semicircle in the high-frequency region and a vertically linear point in the low-frequency region. The high-frequency intercept of the semicircle on the real axis yields the solution (electrolyte) resistance (Rsol), and the diameter of the semicircle yields the charge transfer resistance (Rct) over the interface between the electrode and electrolyte.
In this work, GO, lanthanum sulfide and lanthanum sulfide/GO composite electrodes are successfully deposited by chemical methods. The pseudocapacitive behavior of GO, lanthanum sulfide and composite electrodes is studied in 1 M Na2SO4 electrolyte. The composite electrode showed higher specific capacitance than GO and lanthanum sulfide due to the higher redox activity of composite electrode. The highest specific capacitance obtained for composite electrode is 312 F g−1 at a 5 mV s−1 scan rate. The EIS measurement shows that composite electrode provides low impedance compared with other two electrodes.
Authors are thankful to Department of Science and Technology-Science and Engineering Research Board (DST-SERB), New Delhi, India, for their financial support through research Project No. SERB/F/1677/2016-17 dated January 13, 2017.
Compliance with ethical standards
Conflict of interest
The authors declare that they have no competing interests.
- 9.Ghogare TT, Pujari RB, Lokhande AC, Lokhande CD (2018) Hydrothermally synthesis of nanostructured β-LaS2 thin films. Appl Phys A Mater Sci Process 3:124–248Google Scholar
- 16.Zhang K, Zhang LL, Zhao XS, Wu J (2010) Graphene/polyaniline nanofiber composites as supercapacitor electrode. ACS Chem Mater 22:3509–3516Google Scholar
- 19.Vadiyar MM, Bhise SC, Patil SK, Kolekar SS, Shelke AR, Deshpande NG, Chang JY, Ghule KS, Ghule AV (2013) Contact angle measurement: a preliminary diagnostic tool for evaluating the performance of ZnFe2O4 nano-flake based supercapacitor. J Chem Commun 00:1–3Google Scholar